Two luminescent transition-metal‒organic frameworks with a predesigned ligand as highly sensitive and selective iron(iii) sensors
Zhang, Jian; Zhao, Lili; Liu, Yinxia; Li, Mingyue; Li, Gang; Meng, Xiangru; New Journal of Chemistry 42 (2018) 6839–; doi:10.1039/C8NJ00656C

data_7057173
_publ_section_title
;
 Two luminescent transition-metal--organic frameworks with a predesigned
 ligand as highly sensitive and selective iron(iii) sensors
;
_journal_issue                   9
_journal_name_full               'New Journal of Chemistry'
_journal_page_first              6839
_journal_paper_doi               10.1039/C8NJ00656C
_journal_volume                  42
_journal_year                    2018
_chemical_formula_moiety         'C22 H12 N5 O4 Zn'
_chemical_formula_sum            'C22 H12 N5 O4 Zn'
_chemical_formula_weight         475.74
_space_group_crystal_system      orthorhombic
_space_group_IT_number           20
_space_group_name_Hall           'C 2c 2'
_space_group_name_H-M_alt        'C 2 2 21'
_symmetry_space_group_name_Hall  'C 2c 2'
_symmetry_space_group_name_H-M   'C 2 2 21'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-03-07 deposited with the CCDC.
2018-03-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.4202(11)
_cell_length_b                   14.1684(15)
_cell_length_c                   13.0538(13)
_cell_measurement_reflns_used    2908
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.3946
_cell_measurement_theta_min      3.2653
_cell_volume                     2112.2(4)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0454
_diffrn_reflns_av_unetI/netI     0.0410
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7006
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.495
_diffrn_reflns_theta_min         3.272
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    1.202
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.57538
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'light yellow'
_exptl_crystal_density_diffrn    1.496
_exptl_crystal_description       block
_exptl_crystal_F_000             964
_exptl_crystal_size_max          0.220
_exptl_crystal_size_mid          0.210
_exptl_crystal_size_min          0.200
_refine_diff_density_max         0.553
_refine_diff_density_min         -0.284
_refine_diff_density_rms         0.062
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.41(3)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     173
_refine_ls_number_reflns         1965
_refine_ls_number_restraints     192
_refine_ls_restrained_S_all      1.114
_refine_ls_R_factor_all          0.0414
_refine_ls_R_factor_gt           0.0372
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0591P)^2^+0.6632P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0957
_refine_ls_wR_factor_ref         0.1010
_reflns_Friedel_coverage         0.758
_reflns_Friedel_fraction_full    0.999
_reflns_Friedel_fraction_max     0.999
_reflns_number_gt                1834
_reflns_number_total             1965
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8nj00656c2.cif
_cod_data_source_block           x
_cod_depositor_comments
'Adding full bibliography for 7057172--7057173.cif.'
_cod_database_code               7057173
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.778
_shelx_estimated_absorpt_t_max   0.795
_shelx_res_checksum              72380